### SlideShare for iOS

by Linkedin Corporation

FREE - On the App Store

The International Institute for Science, Technology and Education (IISTE) Journals Call for paper http://www.iiste.org/Journals

The International Institute for Science, Technology and Education (IISTE) Journals Call for paper http://www.iiste.org/Journals

- Total Views
- 332
- Views on SlideShare
- 332
- Embed Views

- Likes
- 0
- Downloads
- 3
- Comments
- 0

No embeds

Uploaded via SlideShare as Adobe PDF

© All Rights Reserved

- 1. Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.3, 2012 Study of Non-Isothermal Kinetic of Austenite Transformation to Pearlite in CK45 Steel by Friedman Model Free Method Mohammad Kuwaiti University of Najaf Abad of Metallurgical Engineering, Iran Tel: +98-09131278784 E-mail: mohammad.kuwaiti@gmail.comAbstractIn recent years, many researchers have been done about the kinetics of thermal decomposition processes. In thisstudy, The Friedman model free method were used to study the Non-Isothermal kinetic of Austenite oTransformation to Pearlite. DTA method was used at cooling rates of 5, 10 and 20 , under argon minatmosphere. Activation energy as a kinetics parameter was determined by using of Friedman model freemethods. The results show that the Activation in Friedman model free method are in range of 40.2-43 KJ . molKeywords: Kinetic, Non-Isothermal, Austenite, Pearlite, Friedman model, DTA, Activation Energy.1. Introduction Heterogeneous chemical reactions are reactions that the components of reaction are in different phases, thesephases that make up the interfaces and usually reactions are performed in interfaces [1]. Reactions are started inAustenite transformation to pearlite from interface of austenite and ferrite. In kinetic study of heterogeneousreactions, is assumed that the equation of rate is also true in the homogeneous gas reactions [2]. In the effect ofcooling, in diagram of equilibrium of Iron – Carbon, austenite transformation to pearlite occurs at thetemperatures near 727 ° C [3, 4]. In this study, Friedman model free method were used for kinetic of austenitetransformation to pearlite in non-isothermal conditions. Using model free methods begin to investigate non-isothermal kinetics from 60 A. D. [5, 6]. In model free methods, is assumed that changing rate of heating thesample, do not change the reaction mechanism and rate reaction is only a function of temperature. Today,determining parameters of kinetics are used by model free methods and the development of equipment [7]. Onthe base, these methods are obtained from STA or DTA [8]. Freeman, Carroll to calculation parameters ofkinetic, use from equation of gases rate, although these equations are correct from the standpoint ofmathematical, but from the standpoint of practical are excited some limitations [9]. In addition, Coats andRedfern use from the approximation of temperature function in integral equations, although this approximationhas some limitation to convert data into logarithms, but it can be a suitable method for the evaluation initial ofthe models of kinetic [10]. Ozawa for calculating the activation energy proposes his own method in a fraction ofthe distinguished converter. In this method, equation 1 is used for calculating activation energy in the variousprogresses fraction of reaction [11]. E (1)ln( β i ) = C − α RTα ,iIn equation 1, C is the constant, Tα ,i is the temperature in the fraction of distinguished progress, R is the gasconstant, βi is cooling rate and Eα is activation energy in the fraction of reaction progress. For calculatingactivation energy in each fraction of the distinguished progress (α ) , changing of Ln β i are drawn vs. 1 and the activation energy is calculated according to slope of the drawn line. Model of fraction of theT αوi converter was proposed by Friedman, in this method, is necessary that the experiments are performed at leastthree different heating rates [5]. In this method, from Equation 2 is used for calculating the activation energy inthe various progresses fraction of reaction. dα E (2)ln β i ( )α = ln[ Af (α )] − ( )α dT RT 24
- 2. Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.3, 2012In this equation, α is the fraction progress of reaction, T is the temperature, R is the gas constant, β i is thecooling rate, A is the pre-exponential factor, f (α ) is the reaction mechanism and E is the activation energy. dα 1For calculating the activation energy in each α , changing ln β i ( )α is drawn vs. and similar dT T αOzawa method, the slope of the drawn lines, will be determined the activation energy. In this study, by usingOzawa and Friedman model free methods, activation energy of austenite transformation to pearlite in CK45 osteel was calculated at cooling rates of 5, 10 and 20 C . min2. Method of research The simple of CK45 steel, with the specified chemical composition in Table 1, was used as basic material.Figure 1 is shown microstructure of the sample which is used. 50 mg samples of the steel was used for the oDTA experiments, by apparatus STA 503, for cooling rates of 5, 10 and 20 C , in non- minisothermal conditions and under argon atmosphere. The used range for the DTA experiments was1200 to 650 o C .3. Results and Discussion oFigure 2 is shown the results of the DTA experiments at cooling rates of 5, 10 and 20 C . minAccording to this figure, the start and finish temperatures of austenite transformation to pearlite arecalculated and with increasing the cooling rate, the starting temperature of transformation is reducedfrom 883 to 679 o C . For calculating the fraction progress of reaction, the area under peak of DTAcurve calculated at any moment and is divided on the area of peak total. Figure 3 shows, the fractionprogress of reaction vs. time at different cooling rates. In this Method, not only parameter of time butalso temperature is important, values of the fraction progress of reaction and the transformationtemperatures were calculated at different cooling rates that are specified in Table 2.As explained in Equation 1, for Calculating activation energy in each fraction of progress should be 1 1 drawn changing of Ln β i vs. . Table 3 shows the values of for the fraction progress T T αوi αوi of reaction in various cooling rates. This information has been calculated by using availableinformation in Figure 3. On this base, with increasing the fraction progress of reaction, reducedactivation energy partially and in addition to Kinetic barriers that exist in the early stages oftransformation, it is justified. It is important that the calculated values of activation energy is theapparent activation energy of transformation and can be included stages of nucleation and growth.Different reports and models in the cases of kinetic of austenite transformation to pearlite have beenpublished But the numerical values is not registered for the activation energy of this transformation[13-17]. It is considered that the mathematical model of Friedmans method (Equation 2) is almost thesame as Ozawa method, but in Friedmans method, rate of transformation be calculated with dα changing of temperature in the fraction progress of reaction ( ( )α ) , be multiplied in the dT cooling rate. Calculating rate of transformation vs. temperature obtain with the numerical method and dα according to the calculated values of α from DTA data. Table 4 shows the values of ln β i ( )α dT in the fraction progress of reaction and for different cooling rates and the corresponding temperature. dαRegarding to Table 4, with increasing the fraction progress of reaction, the values of increase and dT dαalso with increasing the fraction progress of reaction, temperature decrease, the increasing can dTbe reasonably justified, Although reduction of temperature can reduce the diffusion carbon and rates 25
- 3. Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.3, 2012transformation But in this conditions the reduction of temperature cannot impress diffusion and dα 1 austenite rates transformation to pearlite. Figure 4 shows, changing ln β i ( )α vs. in the dT T fraction progress of reaction. In this case, the lines which are drawn are not with a difference slope, sothe expectation is that the values of activation energy which obtained from the Friedman method doesnot change so much with the progress of reaction. Table 5 shows the values of activation energy forthe austenite transformation to pearlite in the fraction progresses of reaction by using the Friedmanmodel and the existing lines which are calculated in Figure 4. From figure 4 can be comprehend thatby the progress of transformation and the increase in the fraction progress of reaction, The activationenergy has a minor fluctuation and change from 43 to 40.2 KJ . The obtained information from molthis method can boost this point that the calculated values of apparent activation energy are largelyclose to the true value. It should be noted that the obtained values for the activation energy of thismethod is not justified on a particular model. However, according to Friedmans equation can multiplyA in f (α ) , but don’t express the model and the reaction mechanism and for calculating the pre-exponential factor of the Friedman model, is necessary to consider f (α ) .References [1] Christian, W., ( 2002): The theory of transformations in metals and alloys , Pergamon, Oxford. [2] Coudurier, L.W., (1970), “Thermodynamics Study of Mo-O-S system”, Trans. Inst. Min. Met., C79, pp.34-40. [3] Mortimer, E., (1979): Chemistry, A Conceptual Approach, Van Nostrand, New York,. [4] Porter, D.A. and Easterling, K.E., (1993): Phase transformations in metals and alloys, Chapman&hall, London. [5] Friedman, H., (1964), "Kinetics of thermal degradation of char-forming plastics from thermogravimetry. Application to a phenolic plastic", Polym. Sci. J., Vol.7, pp. 183–195. [6] Flynn, J.H., (1983 ), “The isoconversional method for determination of energy of activation at constant heating rates”, J. therm. Anal., Vol.27, pp.95-101. [7] Enomoto, M . and Aaronson, H.I., (1986), "Austenite to Ferrite Transformation Kinetics", Metall.trans. A., Vol. 12A, pp. 1547-1557. [8] Kirlcaldy, J.S. and Baganis, (1978), " A computational model for the prediction of steel hardenability", Metall.trans. A., Vol. 9A , pp.495-501. [9] Freeman, E.S., Carroll, B.J., (1958), “The Application of Thermoanalytical Techniques to Reaction Kinetics: The Thermogravimetric Evaluation of the Kinetics of the Decomposition of Calcium Oxalate Monohydrate”, Phys. Chem., Vol. 62, pp.394-397. [10] Coats, A.V. and Redfern, J.P., (1964), “Kinetic Parameters from Thermogravimetric Data”, Nature, 201, pp.68-69. [11] Ozawa, T., (1965), “A New Method of Analyzing Thermogravimetric Data”, Bull. Chem. Soc., Japan., Vol.38, pp.1881-1887. [12] Wegst, C. W., (1989): Stahlschlussel, western, Germany. [13] Hillert, M., Höglund, L., ( 2003), " Reply to comments on kinetics model of isothermal pearlite formation in a 0.4C–1.6Mn steel ", Scripta Mater, Vol. 141, p. 46-78. [14] Kirlcaldy ,J.S., and Baganis, (1978), " A computational model for the prediction of steel hardenability", Metall.trans. A. , Vol. 9A, pp.495-501. [15] Hillert, M., (1962), " Formation of Pearlite Colonies for Simple Models of Alloys Iron-Carbon- Mangenise", Jernkont. Ann., Vol.88, p. 130. [16] Roósz, A.., Gácsi, Z ., Fuchs, E.G., ( 1983), " Isothermal formation of austenite in eutectoid plain carbon steel ", Acta. Metall, Vol. 31, p.509. [17] García de Andrés, C., Alvarez L.F., Carsí, M., (1992), "Modelling of Kinetics and Dilatometric Behavair of Non-Isothermal Pearlite-to-Austenite Transformation in an Eutectoied Steel.", Welding International, Vol.6, p.612. Table 1. Chemical composition of CK45 steel used in this study %Mn %S %P %Si %C steel Heat treatment 0.5-0.8 <0.03 0.35 <0.4 0.42-0.5 CK45 26
- 4. Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.3, 2012 Table 2. Values of the fraction progress of reaction at different cooling rates 5C 10 C 20 C fraction progress of min min min reaction o o o T ( C) T ( C) T ( C) 0.0 883 886 679 0.1 879 882 675 0.2 877 881 672 0.3 876 880 672 0.4 875 879 670 0.5 875 878 669 0.6 874 877 668 0.7 873 876 667 0.8 872 874 666 0.9 871 872 665 1 867 867 662 Table 3. The calculated values by the Ozawa method at different cooling rates Fraction β = 5, ( Lnβ i = 1.609) β = 10, ( Lnβ i = 2.302) β = 20, ( Lnβ i = 3) progress of 1 1 1 reaction T α T α T α 0.1 0.0008679 0.0008654 0.0001054 0.2 0.0008688 0.0008663 0.0001057 0.3 0.0008696 0.0008671 0.0001025 0.4 0.0008704 0.0008679 0.0001060 0.5 0.0008704 0.0008679 0.0001060 0.6 0.0008713 0.0008688 0.0001062 0.7 0.0008721 0.0008696 0.0001063 0.8 0.0008729 0.0008713 0.0001064 0.9 0.0008738 0.0008729 0.0001065 27
- 5. Chemistry and Materials Research www.iiste.org ISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online) Vol 2, No.3, 2012 Table4. The calculated values related to Friedman methods at different cooling rates fractionprogress of β =5 β = 10 β = 20 reaction dα 1 dα 1 dα 1 Ln β i × Ln β i × Ln β i × dT α T α dT α T α dT α T α 0.1 -7.34 0.0008679 -6.64 0.0008654 -6.00 0.0001054 0.2 -6.75 0.0008688 -6.06 0.0008663 -5.30 0.0001057 0.3 -6.33 0.0008696 -5.67 0.0008671 -5.00 0.0001025 0.4 -6.05 0.0008704 -5.31 0.0008679 -4.70 0.0001060 0.5 -5.81 0.0008704 -5.13 0.0008679 -4.40 0.0001060 0.6 -5.64 0.0008713 -4.98 0.0008688 -4.30 0.0001062 0.7 -5.49 0.0008721 -4.81 0.0008696 -4.10 0.0001063 0.8 -5.36 0.0008729 -4.69 0.0008713 -4.00 0.0001064 0.9 -5.25 0.0008738 -4.56 0.0008729 -3.90 0.0001065 Table 5. The values of activation energy for the austenite transformation to pearlite in the obtained fraction progress of reaction by Friedman method Activation Energy( J ) Fraction progress of mol reaction 0.1 42160 0.2 42600 0.3 41686 0.4 40297 0.5 43099 0.6 41337 0.7 41744 0.8 40738 0.9 41162 Figure 1. Microstructure austenite transformation to pearlite of CK45 steel a) 500X b) 100X 28
- 6. Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.3, 2012 Figure 2. Used peaks to calculate the fraction progress of reaction of austenite transformation to pearlite in the o cooling rates (a) 5, (b) 10 and (c) 20 C min Figure 3. The fraction progress of reaction vs. time 29
- 7. Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol 2, No.3, 2012 dα 1 Figure 4. Curves Ln β i × vs. in the fraction progress of reaction 0.1-0.9 dT α T α 30
- 8. This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. Prospective authors ofIISTE journals can find the submission instruction on the following page:http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar

Full NameComment goes here.